#------------------------------------------------------------------------------
#$Date: 2016-03-22 12:05:15 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178933 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/62/4116209.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4116209
loop_
_publ_author_name
'Joanna Goodey'
'Jianggao Mao'
'Arnold M. Guloy'
_publ_section_title
;
 Ba2NiSi3: A One-Dimensional Solid-State Metallocene Analog
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              10478
_journal_page_last               10479
_journal_paper_doi               10.1021/ja0016102
_journal_volume                  122
_journal_year                    2000
_chemical_formula_sum            'Ba2 Ni Si3'
_chemical_formula_weight         417.66
_chemical_name_systematic        Ba2NiSi3
_space_group_IT_number           189
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   11.392(5)
_cell_length_b                   11.392(5)
_cell_length_c                   3.938(3)
_cell_measurement_reflns_used    37
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.27
_cell_measurement_theta_min      2.06
_cell_volume                     442.6(4)
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device       'Siemens Smart 1K CCD'
_diffrn_measurement_method       hemisphere
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1236
_diffrn_reflns_av_sigmaI/netI    0.0745
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            1261
_diffrn_reflns_theta_max         28.27
_diffrn_reflns_theta_min         2.06
_exptl_absorpt_coefficient_mu    16.810
_exptl_absorpt_correction_T_max  1.0
_exptl_absorpt_correction_T_min  0.358
_exptl_absorpt_correction_type   psi
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.701
_exptl_crystal_description       needle
_exptl_crystal_F_000             546
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         1.736
_refine_diff_density_min         -2.070
_refine_diff_density_rms         0.422
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.04(11)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   1.126
_refine_ls_goodness_of_fit_obs   1.133
_refine_ls_matrix_type           full
_refine_ls_number_parameters     23
_refine_ls_number_reflns         411
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.126
_refine_ls_restrained_S_obs      1.133
_refine_ls_R_factor_all          0.0522
_refine_ls_R_factor_obs          0.0502
_refine_ls_shift/esd_max         0.000
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0706P)²+2.0724P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1217
_refine_ls_wR_factor_obs         0.1201
_reflns_number_observed          396
_reflns_number_total             411
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            ja0016102.cif
_cod_data_source_block           Ba2NiSi3_Manuscript_JA0016102-24-131
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0706P)^2^+2.0724P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0706P)^2^+2.0724P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_database_code               4116209
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x, y, -z'
'-y, x-y, -z'
'-x+y, -x, -z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 0.28724(14) 0.0000 0.0000 0.0143(4) Uani 1 d S
Ba2 Ba 0.0000 -0.3819(2) 0.0000 0.0187(5) Uani 1 d S
Ni1 Ni 0.3333 -0.3333 0.0000 0.0159(9) Uani 1 d S
Ni2 Ni 0.0000 0.0000 0.0000 0.0127(12) Uani 1 d S
Si1 Si 0.3161(5) -0.2193(5) -0.5000 0.0140(10) Uani 1 d S
Si2 Si 0.1244(6) 0.1244(6) -0.5000 0.014(2) Uani 1 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Ni2 Ba1 Si1 118.34(9) . 8
Ni2 Ba1 Si1 118.34(9) . .
Si1 Ba1 Si1 123.3(2) 8 .
Ni2 Ba1 Si1 118.34(9) . 8_554
Si1 Ba1 Si1 72.65(11) 8 8_554
Si1 Ba1 Si1 81.2(2) . 8_554
Ni2 Ba1 Si1 118.34(9) . 1_556
Si1 Ba1 Si1 81.2(2) 8 1_556
Si1 Ba1 Si1 72.65(11) . 1_556
Si1 Ba1 Si1 123.3(2) 8_554 1_556
Ni2 Ba1 Si2 42.14(8) . 3
Si1 Ba1 Si2 157.0(2) 8 3
Si1 Ba1 Si2 77.51(12) . 3
Si1 Ba1 Si2 104.22(9) 8_554 3
Si1 Ba1 Si2 117.27(13) 1_556 3
Ni2 Ba1 Si2 42.14(8) . .
Si1 Ba1 Si2 117.27(13) 8 .
Si1 Ba1 Si2 104.22(9) . .
Si1 Ba1 Si2 77.51(12) 8_554 .
Si1 Ba1 Si2 157.0(2) 1_556 .
Si2 Ba1 Si2 41.6(2) 3 .
Ni2 Ba1 Si2 42.14(8) . 1_556
Si1 Ba1 Si2 77.51(12) 8 1_556
Si1 Ba1 Si2 157.0(2) . 1_556
Si1 Ba1 Si2 117.27(13) 8_554 1_556
Si1 Ba1 Si2 104.22(9) 1_556 1_556
Si2 Ba1 Si2 84.3(2) 3 1_556
Si2 Ba1 Si2 69.42(5) . 1_556
Ni2 Ba1 Si2 42.14(8) . 3_556
Si1 Ba1 Si2 104.22(9) 8 3_556
Si1 Ba1 Si2 117.27(13) . 3_556
Si1 Ba1 Si2 157.0(2) 8_554 3_556
Si1 Ba1 Si2 77.51(12) 1_556 3_556
Si2 Ba1 Si2 69.42(5) 3 3_556
Si2 Ba1 Si2 84.3(2) . 3_556
Si2 Ba1 Si2 41.6(2) 1_556 3_556
Ni2 Ba1 Ba2 180.0 . 3_655
Si1 Ba1 Ba2 61.66(9) 8 3_655
Si1 Ba1 Ba2 61.66(9) . 3_655
Si1 Ba1 Ba2 61.66(9) 8_554 3_655
Si1 Ba1 Ba2 61.66(9) 1_556 3_655
Si2 Ba1 Ba2 137.86(8) 3 3_655
Si2 Ba1 Ba2 137.86(8) . 3_655
Si2 Ba1 Ba2 137.86(8) 1_556 3_655
Si2 Ba1 Ba2 137.86(8) 3_556 3_655
Ni2 Ba1 Ba2 73.77(3) . .
Si1 Ba1 Ba2 139.27(7) 8 .
Si1 Ba1 Ba2 60.50(9) . .
Si1 Ba1 Ba2 139.27(7) 8_554 .
Si1 Ba1 Ba2 60.50(9) 1_556 .
Si2 Ba1 Ba2 56.77(10) 3 .
Si2 Ba1 Ba2 97.67(11) . .
Si2 Ba1 Ba2 97.67(11) 1_556 .
Si2 Ba1 Ba2 56.77(10) 3_556 .
Ba2 Ba1 Ba2 106.23(3) 3_655 .
Ni2 Ba1 Ba2 73.77(3) . 2
Si1 Ba1 Ba2 60.50(9) 8 2
Si1 Ba1 Ba2 139.27(7) . 2
Si1 Ba1 Ba2 60.50(9) 8_554 2
Si1 Ba1 Ba2 139.27(7) 1_556 2
Si2 Ba1 Ba2 97.67(11) 3 2
Si2 Ba1 Ba2 56.77(10) . 2
Si2 Ba1 Ba2 56.77(10) 1_556 2
Si2 Ba1 Ba2 97.67(11) 3_556 2
Ba2 Ba1 Ba2 106.23(3) 3_655 2
Ba2 Ba1 Ba2 147.54(6) . 2
Si2 Ba2 Si2 67.72(14) 3_556 3
Si2 Ba2 Ni1 108.32(2) 3_556 .
Si2 Ba2 Ni1 108.32(2) 3 .
Si2 Ba2 Ni1 108.32(2) 3_556 7_545
Si2 Ba2 Ni1 108.32(2) 3 7_545
Ni1 Ba2 Ni1 135.51(5) . 7_545
Si2 Ba2 Si1 142.93(8) 3_556 7_544
Si2 Ba2 Si1 101.40(9) 3 7_544
Ni1 Ba2 Si1 108.72(9) . 7_544
Ni1 Ba2 Si1 39.20(6) 7_545 7_544
Si2 Ba2 Si1 101.40(9) 3_556 2_546
Si2 Ba2 Si1 142.93(8) 3 2_546
Ni1 Ba2 Si1 39.20(6) . 2_546
Ni1 Ba2 Si1 108.72(9) 7_545 2_546
Si1 Ba2 Si1 106.3(2) 7_544 2_546
Si2 Ba2 Si1 101.40(9) 3_556 7_545
Si2 Ba2 Si1 142.93(8) 3 7_545
Ni1 Ba2 Si1 108.72(9) . 7_545
Ni1 Ba2 Si1 39.20(6) 7_545 7_545
Si1 Ba2 Si1 65.18(10) 7_544 7_545
Si1 Ba2 Si1 72.60(15) 2_546 7_545
Si2 Ba2 Si1 142.93(8) 3_556 2_545
Si2 Ba2 Si1 101.40(9) 3 2_545
Ni1 Ba2 Si1 39.20(6) . 2_545
Ni1 Ba2 Si1 108.72(9) 7_545 2_545
Si1 Ba2 Si1 72.60(15) 7_544 2_545
Si1 Ba2 Si1 65.18(10) 2_546 2_545
Si1 Ba2 Si1 106.3(2) 7_545 2_545
Si2 Ba2 Si1 71.99(8) 3_556 1_556
Si2 Ba2 Si1 106.60(9) 3 1_556
Ni1 Ba2 Si1 38.99(6) . 1_556
Ni1 Ba2 Si1 141.99(7) 7_545 1_556
Si1 Ba2 Si1 142.80(5) 7_544 1_556
Si1 Ba2 Si1 38.77(15) 2_546 1_556
Si1 Ba2 Si1 102.79(4) 7_545 1_556
Si1 Ba2 Si1 78.20(11) 2_545 1_556
Si2 Ba2 Si1 106.60(9) 3_556 9_554
Si2 Ba2 Si1 71.99(8) 3 9_554
Ni1 Ba2 Si1 141.99(7) . 9_554
Ni1 Ba2 Si1 38.99(6) 7_545 9_554
Si1 Ba2 Si1 38.77(15) 7_544 9_554
Si1 Ba2 Si1 142.80(5) 2_546 9_554
Si1 Ba2 Si1 78.20(11) 7_545 9_554
Si1 Ba2 Si1 102.79(4) 2_545 9_554
Si1 Ba2 Si1 178.4(2) 1_556 9_554
Si2 Ba2 Si1 106.60(9) 3_556 .
Si2 Ba2 Si1 71.99(8) 3 .
Ni1 Ba2 Si1 38.99(6) . .
Ni1 Ba2 Si1 141.99(7) 7_545 .
Si1 Ba2 Si1 102.79(4) 7_544 .
Si1 Ba2 Si1 78.20(11) 2_546 .
Si1 Ba2 Si1 142.80(5) 7_545 .
Si1 Ba2 Si1 38.77(15) 2_545 .
Si1 Ba2 Si1 64.53(10) 1_556 .
Si1 Ba2 Si1 115.45(10) 9_554 .
Si2 Ba2 Si1 71.99(8) 3_556 9
Si2 Ba2 Si1 106.60(9) 3 9
Ni1 Ba2 Si1 141.99(7) . 9
Ni1 Ba2 Si1 38.99(6) 7_545 9
Si1 Ba2 Si1 78.20(11) 7_544 9
Si1 Ba2 Si1 102.79(4) 2_546 9
Si1 Ba2 Si1 38.77(15) 7_545 9
Si1 Ba2 Si1 142.80(5) 2_545 9
Si1 Ba2 Si1 115.45(10) 1_556 9
Si1 Ba2 Si1 64.53(10) 9_554 9
Si1 Ba2 Si1 178.4(2) . 9
Si1 Ni1 Si1 108.9(2) 1_556 .
Si1 Ni1 Si1 146.19(8) 1_556 2_545
Si1 Ni1 Si1 60.5(2) . 2_545
Si1 Ni1 Si1 60.5(2) 1_556 3_656
Si1 Ni1 Si1 146.19(8) . 3_656
Si1 Ni1 Si1 146.19(8) 2_545 3_656
Si1 Ni1 Si1 60.5(2) 1_556 2_546
Si1 Ni1 Si1 146.19(8) . 2_546
Si1 Ni1 Si1 108.9(2) 2_545 2_546
Si1 Ni1 Si1 60.5(2) 3_656 2_546
Si1 Ni1 Si1 146.19(8) 1_556 3_655
Si1 Ni1 Si1 60.5(2) . 3_655
Si1 Ni1 Si1 60.5(2) 2_545 3_655
Si1 Ni1 Si1 108.9(2) 3_656 3_655
Si1 Ni1 Si1 146.19(8) 2_546 3_655
Si1 Ni1 Ba2 73.52(12) 1_556 .
Si1 Ni1 Ba2 73.52(12) . .
Si1 Ni1 Ba2 72.68(12) 2_545 .
Si1 Ni1 Ba2 125.56(10) 3_656 .
Si1 Ni1 Ba2 72.68(12) 2_546 .
Si1 Ni1 Ba2 125.56(10) 3_655 .
Si1 Ni1 Ba2 72.68(12) 1_556 3_655
Si1 Ni1 Ba2 72.68(12) . 3_655
Si1 Ni1 Ba2 125.56(10) 2_545 3_655
Si1 Ni1 Ba2 73.52(12) 3_656 3_655
Si1 Ni1 Ba2 125.56(10) 2_546 3_655
Si1 Ni1 Ba2 73.52(12) 3_655 3_655
Ba2 Ni1 Ba2 120.0 . 3_655
Si1 Ni1 Ba2 125.56(10) 1_556 2_545
Si1 Ni1 Ba2 125.56(10) . 2_545
Si1 Ni1 Ba2 73.52(12) 2_545 2_545
Si1 Ni1 Ba2 72.68(12) 3_656 2_545
Si1 Ni1 Ba2 73.52(12) 2_546 2_545
Si1 Ni1 Ba2 72.68(12) 3_655 2_545
Ba2 Ni1 Ba2 120.0 . 2_545
Ba2 Ni1 Ba2 120.0 3_655 2_545
Si2 Ni2 Si2 146.04(11) 3 1_556
Si2 Ni2 Si2 108.5(3) 3 3_556
Si2 Ni2 Si2 60.8(2) 1_556 3_556
Si2 Ni2 Si2 60.8(2) 3 2
Si2 Ni2 Si2 146.04(11) 1_556 2
Si2 Ni2 Si2 146.04(11) 3_556 2
Si2 Ni2 Si2 60.8(2) 3 .
Si2 Ni2 Si2 108.5(3) 1_556 .
Si2 Ni2 Si2 146.04(11) 3_556 .
Si2 Ni2 Si2 60.8(2) 2 .
Si2 Ni2 Si2 146.04(11) 3 2_556
Si2 Ni2 Si2 60.8(2) 1_556 2_556
Si2 Ni2 Si2 60.8(2) 3_556 2_556
Si2 Ni2 Si2 108.5(3) 2 2_556
Si2 Ni2 Si2 146.04(11) . 2_556
Si2 Ni2 Ba1 73.02(6) 3 3
Si2 Ni2 Ba1 125.74(13) 1_556 3
Si2 Ni2 Ba1 73.02(6) 3_556 3
Si2 Ni2 Ba1 73.02(6) 2 3
Si2 Ni2 Ba1 125.74(13) . 3
Si2 Ni2 Ba1 73.02(6) 2_556 3
Si2 Ni2 Ba1 73.02(6) 3 .
Si2 Ni2 Ba1 73.02(6) 1_556 .
Si2 Ni2 Ba1 73.02(6) 3_556 .
Si2 Ni2 Ba1 125.74(13) 2 .
Si2 Ni2 Ba1 73.02(6) . .
Si2 Ni2 Ba1 125.74(13) 2_556 .
Ba1 Ni2 Ba1 120.0 3 .
Si2 Ni2 Ba1 125.74(13) 3 2
Si2 Ni2 Ba1 73.02(6) 1_556 2
Si2 Ni2 Ba1 125.74(13) 3_556 2
Si2 Ni2 Ba1 73.02(6) 2 2
Si2 Ni2 Ba1 73.02(6) . 2
Si2 Ni2 Ba1 73.02(6) 2_556 2
Ba1 Ni2 Ba1 120.0 3 2
Ba1 Ni2 Ba1 120.0 . 2
Ni1 Si1 Ni1 108.9(2) 1_554 .
Ni1 Si1 Si1 59.76(8) 1_554 2_545
Ni1 Si1 Si1 59.76(8) . 2_545
Ni1 Si1 Si1 59.76(8) 1_554 3_655
Ni1 Si1 Si1 59.76(8) . 3_655
Si1 Si1 Si1 60.0 2_545 3_655
Ni1 Si1 Ba1 161.87(15) 1_554 .
Ni1 Si1 Ba1 89.23(6) . .
Si1 Si1 Ba1 134.7(2) 2_545 .
Si1 Si1 Ba1 133.8(2) 3_655 .
Ni1 Si1 Ba1 89.23(6) 1_554 1_554
Ni1 Si1 Ba1 161.87(15) . 1_554
Si1 Si1 Ba1 134.7(2) 2_545 1_554
Si1 Si1 Ba1 133.8(2) 3_655 1_554
Ba1 Si1 Ba1 72.65(11) . 1_554
Ni1 Si1 Ba2 120.2(2) 1_554 3_655
Ni1 Si1 Ba2 68.12(9) . 3_655
Si1 Si1 Ba2 121.0(2) 2_545 3_655
Si1 Si1 Ba2 71.3(2) 3_655 3_655
Ba1 Si1 Ba2 65.17(8) . 3_655
Ba1 Si1 Ba2 102.60(14) 1_554 3_655
Ni1 Si1 Ba2 68.12(9) 1_554 3_654
Ni1 Si1 Ba2 120.2(2) . 3_654
Si1 Si1 Ba2 121.0(2) 2_545 3_654
Si1 Si1 Ba2 71.3(2) 3_655 3_654
Ba1 Si1 Ba2 102.60(14) . 3_654
Ba1 Si1 Ba2 65.17(8) 1_554 3_654
Ba2 Si1 Ba2 65.18(10) 3_655 3_654
Ni1 Si1 Ba2 67.49(9) 1_554 1_554
Ni1 Si1 Ba2 119.1(2) . 1_554
Si1 Si1 Ba2 69.9(2) 2_545 1_554
Si1 Si1 Ba2 119.8(2) 3_655 1_554
Ba1 Si1 Ba2 104.78(14) . 1_554
Ba1 Si1 Ba2 67.84(8) 1_554 1_554
Ba2 Si1 Ba2 168.5(2) 3_655 1_554
Ba2 Si1 Ba2 113.87(5) 3_654 1_554
Ni1 Si1 Ba2 119.1(2) 1_554 .
Ni1 Si1 Ba2 67.49(9) . .
Si1 Si1 Ba2 69.9(2) 2_545 .
Si1 Si1 Ba2 119.8(2) 3_655 .
Ba1 Si1 Ba2 67.84(8) . .
Ba1 Si1 Ba2 104.78(14) 1_554 .
Ba2 Si1 Ba2 113.87(5) 3_655 .
Ba2 Si1 Ba2 168.5(2) 3_654 .
Ba2 Si1 Ba2 64.53(10) 1_554 .
Ni2 Si2 Ni2 108.5(3) 1_554 .
Ni2 Si2 Si2 59.61(11) 1_554 3
Ni2 Si2 Si2 59.61(11) . 3
Ni2 Si2 Si2 59.61(11) 1_554 2
Ni2 Si2 Si2 59.61(11) . 2
Si2 Si2 Si2 60.0 3 2
Ni2 Si2 Ba1 64.84(4) 1_554 1_554
Ni2 Si2 Ba1 119.95(12) . 1_554
Si2 Si2 Ba1 69.22(11) 3 1_554
Si2 Si2 Ba1 117.69(11) 2 1_554
Ni2 Si2 Ba1 119.95(12) 1_554 .
Ni2 Si2 Ba1 64.84(4) . .
Si2 Si2 Ba1 69.22(11) 3 .
Si2 Si2 Ba1 117.69(11) 2 .
Ba1 Si2 Ba1 69.42(5) 1_554 .
Ni2 Si2 Ba1 119.95(12) 1_554 2
Ni2 Si2 Ba1 64.84(4) . 2
Si2 Si2 Ba1 117.69(11) 3 2
Si2 Si2 Ba1 69.22(11) 2 2
Ba1 Si2 Ba1 172.7(2) 1_554 2
Ba1 Si2 Ba1 110.09(5) . 2
Ni2 Si2 Ba1 64.84(4) 1_554 2_554
Ni2 Si2 Ba1 119.95(12) . 2_554
Si2 Si2 Ba1 117.69(11) 3 2_554
Si2 Si2 Ba1 69.22(11) 2 2_554
Ba1 Si2 Ba1 110.09(5) 1_554 2_554
Ba1 Si2 Ba1 172.7(2) . 2_554
Ba1 Si2 Ba1 69.42(5) 2 2_554
Ni2 Si2 Ba2 159.6(2) 1_554 2
Ni2 Si2 Ba2 91.88(8) . 2
Si2 Si2 Ba2 135.98(5) 3 2
Si2 Si2 Ba2 135.98(5) 2 2
Ba1 Si2 Ba2 105.34(13) 1_554 2
Ba1 Si2 Ba2 68.29(7) . 2
Ba1 Si2 Ba2 68.29(7) 2 2
Ba1 Si2 Ba2 105.34(13) 2_554 2
Ni2 Si2 Ba2 91.88(8) 1_554 2_554
Ni2 Si2 Ba2 159.6(2) . 2_554
Si2 Si2 Ba2 135.98(5) 3 2_554
Si2 Si2 Ba2 135.98(5) 2 2_554
Ba1 Si2 Ba2 68.29(7) 1_554 2_554
Ba1 Si2 Ba2 105.34(13) . 2_554
Ba1 Si2 Ba2 105.34(13) 2 2_554
Ba1 Si2 Ba2 68.29(7) 2_554 2_554
Ba2 Si2 Ba2 67.72(14) 2 2_554
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 Ni2 3.272(2) .
Ba1 Si1 3.324(4) 8
Ba1 Si1 3.324(4) .
Ba1 Si1 3.324(4) 8_554
Ba1 Si1 3.324(4) 1_556
Ba1 Si2 3.458(2) 3
Ba1 Si2 3.458(2) .
Ba1 Si2 3.458(2) 1_556
Ba1 Si2 3.458(2) 3_556
Ba1 Ba2 3.769(3) 3_655
Ba1 Ba2 3.925(2) .
Ba1 Ba2 3.925(2) 2
Ba2 Si2 3.534(6) 3_556
Ba2 Si2 3.534(6) 3
Ba2 Ni1 3.553(2) .
Ba2 Ni1 3.553(2) 7_545
Ba2 Si1 3.655(5) 7_544
Ba2 Si1 3.655(5) 2_546
Ba2 Si1 3.655(5) 7_545
Ba2 Si1 3.655(5) 2_545
Ba2 Si1 3.688(5) 1_556
Ba2 Si1 3.688(5) 9_554
Ba2 Si1 3.688(5) .
Ba2 Si1 3.688(5) 9
Ni1 Si1 2.420(3) 1_556
Ni1 Si1 2.420(3) .
Ni1 Si1 2.420(3) 2_545
Ni1 Si1 2.420(3) 3_656
Ni1 Si1 2.420(3) 2_546
Ni1 Si1 2.420(3) 3_655
Ni1 Ba2 3.553(2) 3_655
Ni1 Ba2 3.553(2) 2_545
Ni2 Si2 2.426(4) 3
Ni2 Si2 2.426(4) 1_556
Ni2 Si2 2.426(4) 3_556
Ni2 Si2 2.426(4) 2
Ni2 Si2 2.426(4) .
Ni2 Si2 2.426(4) 2_556
Ni2 Ba1 3.272(2) 3
Ni2 Ba1 3.272(2) 2
Si1 Ni1 2.420(3) 1_554
Si1 Si1 2.438(9) 2_545
Si1 Si1 2.438(9) 3_655
Si1 Ba1 3.324(4) 1_554
Si1 Ba2 3.655(5) 3_655
Si1 Ba2 3.655(5) 3_654
Si1 Ba2 3.688(5) 1_554
Si2 Ni2 2.426(4) 1_554
Si2 Si2 2.454(12) 3
Si2 Si2 2.454(12) 2
Si2 Ba1 3.458(2) 1_554
Si2 Ba1 3.458(2) 2
Si2 Ba1 3.458(2) 2_554
Si2 Ba2 3.534(6) 2
Si2 Ba2 3.534(6) 2_554
